- By
**Jimmy** - Follow User

- 1043 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about 'Particle Size Analysis' - Jimmy

Download Now**An Image/Link below is provided (as is) to download presentation**

Download Now

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

Why measure particle size of pharmaceuticals???

Particle size can affect

Final formulation: performance, appearance, stability

“Processability” of powder (API or excipient)

Particle Size AnalysisMicroscopy

Sieving

Sedimentation techniques

Optical and electrical sensing zone method

Laser light scattering techniques

(Surface area measurement techniques)

Methods for determining particle sizeNature of the material to be sized, e.g.

estimated particle size and particle size range

solubility

ease of handling

toxicity

flowability

intended use

Cost

capital

running

Specification requirements

Time restrictions

Choosing a method for particle sizing Optical microscopy (1-150µm)

Electron microscopy (0.001µ-)

Being able to examine each particle individually has led to microscopy being considered as an absolute measurement of particle size.

Can distinguish aggregates from single particles

When coupled to image analysis computers each field can be examined, and a distribution obtained.

Number distribution

Most severe limitation of optical microscopy is the depth of focus being about 10µm at x100 and only 0.5µm at x1000.

With small particles, diffraction effects increase causing blurring at the edges - determination of particles < 3µm is less and less certain.

MicroscopyFor submicron particles it is necessary to use either

TEM (Transmission Electron Microscopy) or

SEM (Scanning Electron Microscopy).

TEM and SEM (0.001-5µm)

Martin's diameter (M)

The length of the line which bisects the particle image. The lines may be drawn in any direction which must be maintained constant for all image measurements.

Feret's diameter (F)

is the distance between two tangents on opposite sides of the particle, parallel to some fixed direction.

Projected area diameter (da or dp)

is the diameter of a circle having the same area as the particle viewed normally to the plane surface on which the particle is at rest in a stable position.

Others:

Longest dimension:

a measured diameter equal to the maximum value of Feret's diameter.

Perimeter diameter:

the diameter of a circle having the same circumference as the perimeter of the particle.

Maximum chord:

a diameter equal to the maximum length of a line parallel to some fixed direction and limited by the contour of the particle.

Types of DiametersManual Optical Microscopy

Advantages

Relatively inexpensive

Each particle individually examined - detect aggregates, 2D shape, colour, melting point etc.

Permanent record - photograph

Small sample sizes required

Disadvantages

Time consuming - high operator fatigue - few particles examined

Very low throughput

No information on 3D shape

Certain amount of subjectivity associated with sizing - operator bias

Transmission and Scanning Electron Microscopy

Advantages

Particles are individually examined

Visual means to see sub-micron specimens

Particle shape can be measured

Disadvantages

Very expensive

Time consuming sample preparation

Materials such as emulsions difficult/impossible to prepare

Low throughput - Not for routine use

Automatic and Image Analysis Microscopes

Advantages

Faster and less operator fatigue than manual

No operator bias

Disadvantages

Can be very expensive

No human judgement retained e.g. to separate out aggregates, select or reject particles etc. (unlike semi-automatic)

Sieve analysis is performed using a nest or stack of sieves where each lower sieve has a smaller aperture size than that of the sieve above it.

Sieves can be referred to either by their aperture size or by their mesh size (or sieve number).

The mesh size is the number of wires per linear inch.

Approx. size range : 5µm - ~3mm

Standard woven wire sieves

Electroformed micromesh sieves at the lower end or range (< 20µm)

Punch plate sieves at the upper range.

SievingSieving may be performed wet or dry; by machine or by hand, for a fixed time or until powder passes through the sieve at a constant low rate

Wet sieving

Air-jet sieving

Weight distribution

Advantages

Easy to perform

Wide size range

Inexpensive

Disadvantages

Known problems of reproducibility

Wear/damage in use or cleaning

Irregular/agglomerated particles

Rod-like particles : overestimate of under-size

Labour intensive

British Pharmacopoeia Volume IV

Appendix XVII A. Particle Size of PowdersParticle size classification of powders

(Ph. Eur. method 2.9.12, Sieve test)

The degree of fineness of a powder may be expressed by reference to sieves that comply with the specifications for non-analytical sieves (2.1.4).

Where the degree of fineness of powders is determined by sieving, it is defined in relation to the sieve number(s) used either by means of the following terms or, where such terms cannot be used, by expressing the fineness of the powder as a percentage m/m passing the sieve(s) used.

The following terms are used in the description of powders:

Coarse powder: Not less than 95% by mass passes through a number 1400 sieve and not more than 40 % by mass passes through a number 355 sieve.

Moderately fine powder: Not less than 95% by mass passes through a number 355 sieve and not more than 40% by mass passes through a number 180 sieve.

Fine powder: Not less than 95% by mass passes through a number 180 sieve and not more than 40% by mass passes through a number 125 sieve.

etc., etc….

Methods depend on the fact that the terminal velocity of a particle in a fluid increases with size.

Stokes's Law :

Stokes's diameter (dst) is defined as the diameter of the sphere that would settle at the same rate as the particle

Sedimentation techniquesThe particle size distribution of fine powder can be determined by examining a sedimenting suspension of the powder.

2 categories:

(1) Incremental : changes with time in the concentration or density of the suspension at known depths are determined. Can be either fixed time or fixed depth techniques.

(2) Cumulative : the rate at which the powder is settling out of suspension is determined. i.e the accumulated particles are measured at a fixed level after all particles between it and the fluid's surface have settled.

Weight distribution

Size distribution is determined by allowing a homogeneous suspension to settle in a cylinder and taking samples from the settling suspension at a fixed horizontal level at intervals of time.

Each sample will contain a representative sample of the suspension, with the exception of particles greater than a critical size, all of which will have settled below the level of the sampling point.

The concentration of solid in a sample taken at time t is determined by centrifugation of the sample followed by drying and weighing or simply by drying and weighing.

This concentration expressed as a percentage of the initial concentration gives the percentage (w/w) of particles whose falling velocities are equal to or less than x/t. Substitution in the equation above gives the corresponding Stokes' diameter.

Andreasen PipetteAdvantages

Equipment required can be relatively simple and inexpensive.

Can measure a wide range of sizes with considerable accuracy and reproducibility.

Disadvantages

Sedimentation analyses must be carried out at concentrations which are sufficiently low for interactive effects between particles to be negligible so that their terminal falling velocities can be taken as equal to those of isolated particles.

Large particles create turbulence, are slowed and are recorded undersize.

Careful temperature control is necessary to suppress convection currents.

The lower limit of particle size is set by the increasing importance of Brownian motion for progressively smaller particles.

Particle re-aggregation during extended measurements.

Particles have to be completely insoluble in the suspending liquid.

Instrument measures particle volume which can be expressed as dv : the diameter of a sphere that has the same volume as the particle.

The number and size of particles suspended in an electrolyte is determined by causing them to pass through an orifice an either side of which is immersed an electrode.

The changes in electric impedance (resistance) as particles pass through the orifice generate voltage pulses whose amplitude are proportional to the volumes of the particles.

Volume distribution

Electrical sensing zone method – Coulter CounterObscuration of light source relates to particle size (area)

Advantage of not requiring medium to be an electrolyte

Optical sensing zone methodLaser Diffraction Particle Size Analysis

(Particle size range 0.02-2000µm)

Photon Correlation Spectroscopy

(Particle size range :1nm to 5µm)

Laser light scattering techniquesParticles pass through a laser beam and the light scattered by them is collected over a range of angles in the forward direction.

The angles of diffraction are, in the simplest case inversely related to the particle size.

The particles pass through an expanded and collimated laser beam in front of a lens in whose focal plane is positioned a photosensitive detector consisting of a series of concentric rings.

Distribution of scattered intensity is analysed by computer to yield the particle size distribution.

Laser diffraction- Volume distribution

Advantages:

Non-intrusive : uses a low power laser beam

Fast : typically <3minutes to take a measurement and analyse.

Precise and wide range - up to 64 size bands can be displayed covering a range of up to 1000,000:1 in size.

Absolute measurement, no calibration is required. The instrument is based on fundamental physical properties.

Simple to use

Highly versatile

Disadvantages:

expense

volume measurement all other outputs are numerical transformations of this basic output form, assuming spherical particles

must be a difference in refractive indices between particles and suspending medium

Large particles move more slowly than small particles, so that the rate of fluctuation of the light scattered from them is also slower.

PCS uses the rate of change of these light fluctuations to determine the size distribution of the particles scattering light.

Comparison of a "snap-shot" of each speckle pattern with another taken at a very short time later (microseconds).

The time dependent change in position of the speckles relates to the change of position of the particles and hence particle size.

The dynamic light signal is sampled and correlated with itself at different time intervals using a digital correlator and associated computer software.

The relationship of the auto-correlation function obtained to time intervals is processed to provide estimates of the particle size distribution.

PCSAdvantages:

Non-intrusive

Fast

Nanometre size range

Disadvantages:

Sample prep critical

Vibration, temperature fluctuations can interfere with analysis

Restricted to solid in liquid or liquid in liquid samples

Expense

Need to know R.I. values and viscosity

Download Presentation

Connecting to Server..